#------------------------------------------------------------------------------
#$Date: 2023-05-23 11:35:25 +0300 (Tue, 23 May 2023) $
#$Revision: 283960 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/18/9001895.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9001895
loop_
_publ_author_name
'Tribaudino, M.'
'Benna, P.'
'Bruno, E.'
_publ_section_title
;Structural variations induced by thermal treatment in lead feldspar
 (PbAl2Si2O8) Sample: PbF_L16h, single Pb site
;
_journal_name_full               'American Mineralogist'
_journal_page_first              159
_journal_page_last               166
_journal_volume                  83
_journal_year                    1998
_chemical_formula_sum            'Al2 O8 Pb Si2'
_chemical_name_mineral           Feldspar
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-I 2yc'
_symmetry_space_group_name_H-M   'I 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.28
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.399
_cell_length_b                   13.061
_cell_length_c                   14.334
_cell_volume                     1421.841
_database_code_amcsd             0001955
_exptl_crystal_density_diffrn    4.161
_cod_original_formula_sum        'Pb (Al2 Si2) O8'
_cod_database_code               9001895
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
1/2+x,1/2+y,1/2+z
x,-y,1/2+z
1/2+x,1/2-y,+z
-x,y,1/2-z
1/2-x,1/2+y,-z
-x,-y,-z
1/2-x,1/2-y,1/2-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_type_symbol
_atom_site_attached_hydrogens
Pb 0.27230 -0.00790 0.07190 1.00000 Pb 0
Al1o 0.00720 0.17730 0.10970 0.14000 Al 0
Si1o 0.00720 0.17730 0.10970 0.86000 Si 0
Al1z 0.00250 0.17930 0.61530 0.86000 Al 0
Si1z 0.00250 0.17930 0.61530 0.14000 Si 0
Al2o 0.69580 0.11980 0.17140 0.86000 Al 0
Si2o 0.69580 0.11980 0.17140 0.14000 Si 0
Al2z 0.68750 0.11490 0.67380 0.14000 Al 0
Si2z 0.68750 0.11490 0.67380 0.86000 Si 0
OA(1) 0.00200 0.13450 -0.00100 1.00000 O 0
OA(2) 0.59840 -0.00040 0.14650 1.00000 O 0
OB(o) 0.82940 0.12940 0.10790 1.00000 O 0
OB(Z) 0.81480 0.13220 0.61630 1.00000 O 0
Oc(o) 0.01790 0.30080 0.12190 1.00000 O 0
Ocz 0.02000 0.31050 0.63250 1.00000 O 0
Odo 0.18370 0.12440 0.19630 1.00000 O 0
Odz 0.19860 0.12280 0.70210 1.00000 O 0
loop_
_cod_changelog_entry_id
_cod_changelog_entry_author
_cod_changelog_entry_date
_cod_changelog_entry_text
1
;cod-tools version 3.8.0
Id: cif_guess_AMCSD_atom_types 9581 2023-05-17 12:35:41Z saulius
;
2023-05-23T09:16:18+03:00
;Derived atom types and hydrogen counts
from atom names that follow the AMCSD naming convention
(Wat == water, O-H == hydroxyl).
;
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0001955
